**HAL Id: hal-00771744**

**https://hal.archives-ouvertes.fr/hal-00771744**

### Submitted on 9 Jan 2013

**HAL is a multi-disciplinary open access**

### archive for the deposit and dissemination of

### sci-entific research documents, whether they are

### pub-lished or not. The documents may come from

### teaching and research institutions in France or

### abroad, or from public or private research centers.

**L’archive ouverte pluridisciplinaire HAL, est**

### destinée au dépôt et à la diffusion de documents

### scientifiques de niveau recherche, publiés ou non,

### émanant des établissements d’enseignement et de

### recherche français ou étrangers, des laboratoires

### publics ou privés.

**In-plane magnetic penetration depth in NbS2**

### Pascale Diener, Maxime Leroux, Laurent Cario, Thierry Klein, Pierre Rodiere

**To cite this version:**

### Pascale Diener, Maxime Leroux, Laurent Cario, Thierry Klein, Pierre Rodiere. In-plane magnetic

### penetration depth in NbS2. Physical Review B: Condensed Matter and Materials Physics (1998-2015),

### American Physical Society, 2011, 84 (5), pp.054531. �10.1103/PhysRevB.84.054531�. �hal-00771744�

### In-plane magnetic penetration depth in NbS

_{2}

P. Diener1_{, M. Leroux}1_{, L. Cario}2_{, T. Klein}1,3_{, P. Rodière}1
1

Institut Néel, CNRS/UJF 25 rue des Martyrs BP 166 38042 Grenoble cedex 9, FRANCE

2

Institut des Matériaux Jean Rouxel (IMN), Université de Nantes, CNRS, 2 rue de la Houssinière, BP3229, 44322 Nantes, France and

3

Institut Universitaire de France and Université J.Fourier-Grenoble 1, France

We report on the temperature dependence of the in plane magnetic penetration depth (λab)

and first penetration field (Hf ∝ 1/λ 2

ab(T ) for Hkc) in 2H-NbS2 single crystals. An exponential

temperature dependence is clearly observed in λab(T) at low temperature, signing the presence of

a fully open superconducting gap. This compound is the only superconducting 2H-dichalcogenide which does not develop a charge density wave (CDW). However as previously observed in 2H-NbSe2,

this gap ( ∆1 = 1.1 kBTc) is significantly smaller than the standard BCS weak coupling value. At

higher temperature, a larger gap (∆2= 1.8 kBTc) has to be introduced to describe the data which

are compatible with a two gap model. The superconducting gaps are hence very similar in NbS2

and NbSe2 and we show here that both of them open in the strongly coupled Nb tubular sheets

independently of the presence of a CDW or not.

I. INTRODUCTION

In numerous strongly correlated systems,
superconduc-tivity appears in the vicinity of a second electronic
in-stability. These superconductors then often show
devi-ations from the weak coupling BCS theory which raises
the question of the interplay between the two orders1_{.}

This question is particularly well illustrated in dichalco-genides. Indeed, in 1T-TiSe22,3, 2H-TaS24,5, or

2H-NbSe2 superconductivity coexists with a charge density

wave (CDW). In 2H-NbSe2 the charge density wave

de-velops for instance at TD = 33 K and coexists with

su-perconductivity (SC) below Tc= 7.1 K.

In parallele, specific heat, tunneling spectroscopy as
well as de Haas van Alphen measurements6–10 _{showed}

that NbSe2is characterized by the coexistence of two

su-perconducting gaps : ∆1= 1.0 ± 0.1kBTc which is much

smaller than the BCS weak coupling value (∆/kBTc ∼

1.7) and ∆2 = 2.0 ± 0.3kBTc. It was then initially

sug-gested that the CDW might be at the origin of ∆111–14.

However, scanning tunneling spectroscopy (STS) and specific heat measurements clearly indicated the pres-ence of a reduced superconducting gap (of similar am-plitude) in the NbS2 system as well15,16 showing that

this interpretation does not hold the ground. Indeed,
this iso-electronic compound is particularly interesting
to probe the possible influence of the CDW on the
superconducting states in dichalcogenides, as it is the
only system among the four 2H layered
superconduct-ing transition-metal dichalcogenides17 _{MX}

2 (M=Nb,Ta;

X=S, Se) which does not exhibit a CDW transition. Those measurements hence clearly showed that the pres-ence of two superconducting gaps in 2H-dichalcogenides is not a direct consequence of the presence of a CDW in some of them.

In a first scenario, those two gaps can be considered as being the limiting values of one single anisotropic su-perconducting gap (without nodes) whereas in an alter-native scenario they can be related to different values of the electron phonon coupling constants (λe−ph) on

differ-ent sheets of the Fermi surface (FS) (so called multiband
superconductivity18_{).}

Clear evidence for multiband superconductivity were first obtained in MgB2for which λe−phvaries from ∼ 1.2

for the 2D-σ band to ∼ 0.4 for the 3D-π band19,20_{. Since}

the FS of NbSe2 is composed of four strongly coupled

quasi-2D Nb-derived cylinders (bands 17 and 18 with λe−ph ranging from 0.8 to 1.9) and one Se-derived

pan-cake sheet with a much smaller λe−ph value ∼ 0.3 (band

16)8_{, it was tempting to ascribe the small }

superconduct-ing gap to this reduced λe−ph21,22. However ARPES

measurements11,14 _{suggested that, in NbSe}

2, both gaps

open on the tubular sheets and the situation iseems to be quite different from that of MgB2 as the two gaps

could both be associated to the same (strongly coupled) FS sheets. However, an experimental confirmation that the tow gaps are also related to the same FS sheets in NbS2 was still lacking.

In order to address this issue, we have performed in plane penetration depth and penetration field measure-ments in NbS2 single crystals. Indeed, λ is a directional

probe and corresponding measurements are only sensitive to supercurrents flowing perpendicularly to the direction of the applied magnetic field. Band structure calculations in NbSe2have for instance shown that the tubular sheets

contribute to 98% of the transport current in the basal
plane23_{, and the present measurements will hence only}

probe the superconducting properties of those strongly couple sheets. We show here that the temperature de-pendence of λab are remarkably identical in NbSe2 and

NbS2. This temperature dependence clearly confirms the

presence of a small superconducting gap ∆1 = 1.1 kBTc

(being much smaller than the standard BCS weak cou-pling value) and that, as previously observed in NbSe2,

this gap opens on as least one of the Nb sheets. At higher temperature the superfluid density can be deduced from λ(T ) introducing a calibration factor (see below) which can be accurately obtained combining λ(T ) and first pen-etration field measurements. We then also show that a second gap value is required to describe the

tempera-ture dependence of this superfluid density which can be well described by a two gap model introducing gap values very similar to those previously obtained in specific heat measurements. We hence confirm that the presence of two well defined superconducting gap values, both open-ing on the Nb tubular sheets in a generic feature of 2H-dichalconenides.

STS and specific heat (Cp) measurements clearly

showed that NbSe2 and NbS2 systems share the

par-ticularity of having both two superconducting gaps but also highlighted some fundamental differences. Indeed, whereas vortices exhibit a clear stellar shape in NbSe2,

they appear to be isotropic in NbS2. Moreover, the two

systems have very different anisotropies of their upper critical fields increasing from ∼ 3.2 in NbSe29to ∼ 8.1 in

NbS224. However, the vortex shape and Hc2 values are

determined by the coherence length (ξ) which is related to the superconducting gap but also to electronic prop-erties of the normal state (Fermi velocity and possibly electronic mean free path in the so-called dirty limit). On the contrary the temperature dependence of the pen-etration depth is determined only by the superconducting gap structure. Those later measurements hence provide very valuable information to understand those differences which will be discussed at the end of the paper.

II. SAMPLE AND EXPERIMENTS

2H-NbS2 samples were grown using the vapour

trans-port growth technique with a large sulphur excess, as
described elsewhere25_{. Single crystals have a flat }

hexag-onal or triangular shape and typical dimensions of 1502_{×}

30 µm. The large flat faces grow perpendicular to the
c-axis. The 2H crystallographic structure has been checked
on each sample using a four-circle diffractometer. The
bulk critical temperature was checked on several
sam-ples of each batch by ac specific heat16_{. All the }

mea-sured crystals showed sharp superconducting transitions (∆Tc∼ 0.3 K) at Tc= 6.05±0.2 K emphasizing the

excel-lent bulk homogeneity of each crystal. Previous scanning
tunnelling microscopy measurements on single crystals of
the same origin confirmed the absence of CDW down to
0.1 K15_{. To avoid a contamination by oxygen }

intercala-tion between layers which would reduce Tc and smears

the transition24_{, samples were kept in vacuum. All the}

measurements were carried out in the first month follow-ing the growth of the samples.

A high stability LC oscillator operating at 14 MHz,
driven by a Tunnel Diode26–28_{has been used to measure}

the variation of the magnetic penetration depth. The tiny sample, placed in the center of the solenoid coil, acts as a small perturbation to the inductance (L). By chang-ing the temperature of the sample, the magnetic penetra-tion depth variapenetra-tions produce a change of the inductance, leading to a change in the LC resonant frequency δf(T ). The amplitude of the AC excitation field is smaller than 1µT (that is «Hc1) to keep the sample in the Meissner

Figure 1: Temperature dependence of the frequency shift δf (T), for B (square) D (triangle) (right scale)and C8 (cir-cle) (left scale)NbS2 single crystals. Inset: microscope images

of each sample (note the bigger scale for C8).

state. This technique enables to measure the variation of λ with an excellent sensitivity as our setup can detect relative frequency changes, δf/f0 of a few 10−9, which

corresponds to changes in λ on the order of 1 Åin mm3

samples. The sample is glued with vacuum grease at the bottom of a sapphire cold finger whose temperature is regulated between Tmin=0.5 K and 10 K whereas the

LC oscillator remains at fixed temperature (3K). The fre-quency shift δf=f(T ) − f(Tmin) is then proportional to

the magnetic penetration depth : δλ(T ) = Rδf (T )

∆f0

(1) where ∆f0 is the change induced by the introduction of

the superconducting sample in the coil (measured in-situ
by extracting the cold finger from the coil at the
low-est temperature), and R an effective dimension which
depends on the sample geometry. In principle, R can
be evaluated by using the formula proposed by Prozorov
and al.29 _{in the case of cylinders. However, recent }

mea-surements in pnictides highlighted the difficulties of
eval-uating this effective dimension, in particular for
mag-netic fields perpendicular to the ab-planes (main sample
surface)30_{. Indeed, very different δλ(T ) were obtained by}

different groups, most probably due to the roughness of the sample edges which undermines this evaluation.

To overcome this difficulty we have performed first pen-etration field (Hf) measurements using miniature

GaAs-based quantum well Hall probe arrays. The remanent local DC field (Brem(Ha)) in the sample has been

mea-sured after applying a magnetic field Ha and sweeping

the field back to zero. In the Meissner state, no vortices penetrate the sample and Brem remains equal to zero up

to Ha = Hf. A finite Brem value is then obtained for

Ha ≥ Hf due to vortices which remain pinned in the

sample. As Hf is directly proportional to the first

cal field Hc1∝ 1/λ2, the normalized in plane superfluid density : ˜ ρab(T ) = λ 2 0 λ2 ab(T ) = 1 (1 + R λ0∆f0δf (T )/) 2 (2)

is expected to vary as Hf(T )/Hf(0) (λ0 being the zero

temperature penetration depth). Even though the un-certainties on the Hf values hinders any precise

determi-nation of the gap values, those measurements can then be used as milestones to obtain the R/λ0∆f0 coefficient

(see inset of Fig.3).

III. EVIDENCE FOR A SMALL GAP VALUE IN

NBS2

Fig. 1 shows typical δf(T ) curves between 0.08 Tc

and 0.85 Tc for three NbS2 single crystals (see inset of

Fig. 1). The magnetic field is applied perpendicularly to the layers, i.e. along the crystallographic c axis, so that supercurrents are flowing in the layers, probing the in-plane penetration depth, λab31. Samples B and D were

grown in the same batch, and have, in-plane dimensions
equal to 110 µm and 140µm, respectively and a
thick-ness t = 30µm (resp. 25µm). Sample C8 was grown in
a second batch and has a larger size (4302_{× 110 µm}3_{).}

The frequency shift is ten times higher for C8 than for other samples due to it larger volume but all renormal-ized curves are fully identical underlying the excellent reproducibility of the temperature dependence discussed below.

In the local London theory, at low temperature (typi-cally T < Tc/3), the temperature dependence of the gap

can be neglected and λ(T ) is given by : (λ(T ) − λ0)/λ0=

s π∆(0)

2kBT

e−∆(0)/kBT (3)

where kB is the Boltzmann constant and ∆(0) the value

of the smallest superconducting gap at 0 K. Indeed, due to this exponential dependence only the smallest gap is expected to show up at low temperature. As shown in Fig.2 a very poor agreement to the data is obtained if the gap parameter is fixed to the weak coupling BCS gap of 1.76kBTc. A much better fit is obtained taking

∆/kB = 7.2 K≈ 1.2 Tc. Note that this gap value does

not depend on the renormalization constant. The as-sumption λ(Tmin) ≈ λ0, where Tminis the lowest

exper-imental temperature, is valid here, since an extrapolation of Eq.(3) gives (λ(0.5K) − λ0)/λ0< 10−3. Since the

su-perfluid current mainly originates from the Nb sheets for Hkc, those measurements hence directly show that this small gap is associated with those sheets in NbS2as well.

In order to get information on the larger gap, it is nec-essary to perform a detailed analysis of the temperature dependence at higher temperature. The inset of fig.3 displays the temperature dependence of the-superfluid

Figure 2: Temperature dependence of the rescaled frequency shift δf /∆f0 ∝ ∆λab/λ0 in NbS2 at T<Tc/3 (red circles).

Results are fitted with the exponential low temperature ap-proximation (see text) to determine the smaller gap ∆. An excellent fit is obtained for ∆ ≈ 1.17 kBTc. Results can’t be

described by an exponential behaviour with the weak coupling BCS value ∆ = 1.76 kBTc. Inset: superconducting transition:

Tc=6.05 K is determined by the maximum of variation of the

frequency shift.

density ˜ρab(T ) up to Tc deduced from Eq.(2) for

differ-ent R/λ0∆f0 values compared to Hf/Hf(0). Note that

if a small change in R/λ0∆f0 will modify strongly the

normalized superfluid density, the curvature of Hf(T) is

utterly independent of λ0. Hf(T) can hence be used to

determine R/λ0∆f0with good accuracy and, as shown, a

good agreement between Hfand the superfluid density is

obtained taking R/λ0∆f0= 0.02Hz−1. Clear deviations

from the BCS weak coupling theoretical curve (dashed line) is visible on the entire temperature range. In par-ticular, the BCS values exceed the experimental data at low temperature due to the small value of the gap.

In the multigap model, ˜ρ is phenomenologically as-sumed to be the sum of two independent superfluid den-sities

˜

ρ = ω ˜ρ1+ (1 − ω) ˜ρ2 (4)

where ω is the weight of band 1 and ˜ρi are given by

˜
ρi(T ) = 1 −
Z _{∂f}
∂E
E
pE2_{− ∆}2
i(T )
(5)
The best fit to the data using Eq.(4) and Eq.(5) (solid
line in Fig.3) is obtained with ∆1= 1.05±0.05×kBTcand

∆2= 1.8 ± 0.1 × kBTc with ω ∼ 0.5. Those values are in

very good agreement with those deduced from tunneling spectroscopy measurements which revealed a distribution of gaps having two main values at 0.53 meV=6.15 K≈ 1 kBTcand 0.98 meV=10.8 K≈ 1.8 kBTc15. Moreover, the

Figure 3: Normalized superfluid density of NbS2

de-duced from Tunnel Diode Oscillator measurements (TDO) for Rλ0/∆f0=0.02Hz−

1

(closed squares), compared to Hf(T )/Hf(0)(open circles) both on sample C8. As shown,

the weak coupling BCS normalized superfluid density (dashed line) is not compatible with the data. A very similar tem-perature dependence was previously obtained in NbSe2 (solid

triangles) and both compounds could be well described by a two gap model (thick line, see text for details). Inset: influence of the R/λ0∆f0 parameter on the shape of the superfluid

den-sity, R/λ0∆f0 being equal to respectively 0.01, 0.02 and 0.03

Hz−1 _{for diamonds, squares and circles.}

sample C8 can be well described taking ∆1∼ 1.05×kBTc,

∆2 ∼ 2.1 × kBTc and ω ∼ 0.616. Even if this two gap

model well reproduces the temperature dependence of ˜ρi

it is worth noting that this temperature dependence is
also compatible with a single anisotropic in-plane
super-conducting gap. The simplest model which respects the
symmetry of the crystal has an in-plane 6-fold shape,
∆(φ) = ∆1+∆2−∆_{2} 1(1 + cos(6φ)) where the extremum

of the superconducting gap define two characteristics en-ergy scales. With this model, we find ∆1∼ 0.9(1)× kBTc

and ∆2∼ 1.9(3) × kBTc.

IV. _{COMPARISON BETWEEN NBS}2 AND

NBSE2

We have also reported in Fig.3 the temperature depen-dence of ˜ρab deduced from penetration depth

measure-ments in 2H-NbSe212. Since the critical temperatures

are slightly different in the two compounds, the data have been plotted as a function of T/Tcwith Tc= 6.05 K and

7.1 K for NbS2and NbSe2, respectively. In both case, the

presence of two characteristic gap values are necessary to fit the temperature dependence of the in-plane superfluid density. We hence show that in both compounds the ex-otic superconducting gap structure is related to the Nb tubular sheets and that, even if the charge density wave is

perturbing those sheets in NbSe2(but not in NbS2which

does not exhibit any CDW), this CDW does not affect the superconducting gap structure. Our results hence contradict the ARPES measurements on NbSe211which

suggested a strong correlation between the gap structure and the CDW formation. The presence of an identical exotic gap structure in two different compounds (even of the same family) is particularly rare which highlights the robustness of the underlying mechanism at its ori-gin. It’s worth noting that there exists a R/λ0∆f0value

(∼ 0.02Hz−1_{, see above) for which the temperature }

de-pendence obtained on both compounds are very similar on the whole temperature range.

Note that this strong similitude in the gap structure is not in contradiction with the fact that the vortex cores have an isotropic shape in NbS215, and 6-fold shape in

NbSe232,33. Indeed, in this later case, the particular

shape could be due to an anisotropic Fermi velocity34

caused by the presence of the Charge Density Wave. Finally, It is interesting to note that even with sim-ilar superconducting gaps, it is possible to understand the large difference of the anisotropy of the upper crit-ical field in the two systems. In the case of NbSe2,

the anisotropy of the upper critical field can be
under-stood by the anisotropy of the two set of Nb-bands.
In-deed, the coherence length related to the pancake band
is larger due to a large renormalised Fermi velocity and
a small gap8_{. According to band structure calculations,}

the anisotropy of the Fermi velocities (vab

F/vFc) of the two

tubular sheets are on the order of 2 (Band 1735_{) and 10}

(Band 18) in NbSe2, none of which corresponding to the

experimental value of the anisotropy of the upper
crit-ical field (∼ 3.2)23_{. However, µ}

0Hc2kc(0) = Φ0/2πξab2 is

defined by the band having the smallest ξab value. All

bands have quite similar in plane Fermi velocities but if one assumes that ∆2 is associated with band 17 and ∆1

to band 18, on gets ξab,17 ∼ (∆1/∆2)ξab,18 ∼ ξab,18/1.7

and Hkc

c2 will be defined by band 17. Moreover, for

µ0Hc2kab(0) = Φ0/2πξabξc, and the very small value of

c-axis Fermi velocity of band 18, will imply that Hkab c2

will be defined by this latter band. One hence gets Hc2kab/H kc c2 = (v ab,17 F .v ab,17 F /v ab,18 F .v c,18 F ) × (∆1/∆2)2 ∼

10/(1.7)2 _{∼ 3 in good agreement with the }

experimen-tal value. Note that this situation strongly differs from the one observed in MgB2in which the anisotropy of Hc2

is defined only by the σ−band (for T << Tc). As NbSe2

and NbS2 have similar Hc2kab values, one can conclude

that band 18 is not affected by the chemical substitution and the increase of the Hc2 anisotropy to ∼ 8.1 in NbS2

is a hence due to an increase of vab,17

F but this change in

the Fermi velocity does not affect the superconducting gap structure.

The presence of two characteristics gap values appears to be a robust characteristic feature in 2H dichalco-genides, but its origin is still open to questions. With the present results, the influence of the CDW also has to be excluded, underlying the necessity to propose new 4

clues for the origin of the reduced superconducting gap observed in both compounds.

V. CONCLUSION

To conclude, the temperature dependence of the in-plane magnetic penetration depth of single crystals of 2H-NbS2 has been measured, and compared to previous

measurements on 2H-NbSe2. The temperature

depen-dence shows a similar curvature in both compounds evi-dencing a similar reduced superconducting gap structure in the sheets of the Fermi Surface where the e-ph

cou-pling constant are the largest. The CDW, present only in NbSe2, is not at the origin of the reduced

supercon-ducting gap. In the light of the discovery of a particular
acoustic phonon mode observed in lead or Niobium36_{,}

a more accurate knowledge of the phonon dispersion in NbS2 could shed insight into the origins of the reduced

superconducting gap in the dichalcogenides.

P.R. thanks R. and B. Thomas for helpful discussions. . TK is most obliged to V. Mosser of ITRON, Montrouge, and M.Konczykowski from the Laboratoire des Solides Ir-radiés, Palaiseau for the development of the Hall sensors used in this study

1

G. Seyfarth, J. P. Brison, and G. K. et al., Phys. Rev. Lett.
101_{, 046401 (2008).}

2

E. Morosan, H. W. Zandbergen, and B. S. e. a. Dennis, Nature Physics 2, 544 (2006).

3

A.F. Kusmartseva, B. Sipos, H. Berger, L. Forro, E. Tutis, Phys. Rev. Lett. 103, 236401 (2009).

4

B. Sipos, A. Kusmartseva, and A. A. et al., Nature Mate-rials 7, 960 (2008).

5

K. E. Wagner, E. Morosan, Y. S. Hor, J. Tao, Y. Zhu, T. Sanders, T. M. McQueen, H. W. Zandbergen, A. J. Williams, D. V. West, et al., Phys. Rev. B 78, 104520 (2008).

6

P. Garoche, J. J. Veyssié, P. Manuel, and P. Molinié, Solid. State Comm. 19, 455 (1976).

7

H. F. Hess, R. B. Robinson, R. C. Dynes, J. M. Valles, and J. V. Waszczak, Phys. Rev. Lett. 62, 214 (1989).

8

R. Corcoran, P. Meeson, Y. Onuki, P. A. Probst, M. Springford, K. Takita, H. Harima, G. Y. Guo, and B. L. Gyorffy, J. Phys.: Condens. Matter 6, 4479 (1994).

9

D. Sanchez, A. Junod, J. Muller, H. Berger, and F. Lévy, Physica B 204, 167 (1995).

10

I. Guillamon, H. Suderow, F. Guinea, and S. Vieira, Phys. Rev. B 77, 134505 (2008).

11

T. Kiss, T. Yokoya, A. Chainani, S. Shin, T. Hanaguri, M. Nohara, and H. Takagi, Nat. Phys. 3, 720 (2007).

12

J. D. Fletcher, A. Carrington, P. Diener, P. Rodiere, J. P. Brison, R. Prozorov, T. Olheiser, and R. W. Giannetta, Phys. Rev. Lett. 98, 057003 (2007).

13

A. H. Castro Neto, Phys. Rev. Lett. 86, 4382 (2001).

14

S. V. Borisenko, A. A. Kordyuk, V. B. Zabolotnyy, D. S. Inosov, D. Evtushinsky, B. Büchner, A. N. Yaresko, A. Varykhalov, R. Follath, W. Eberhardt, et al., Phys. Rev. Lett. 102, 166402 (2009).

15

I. Guillamon, H. Suderow, S. Vieira, L. Cario, P. Diener, and P. Rodiere, Phys. Rev. Lett. 101, 166407 (2008).

16

J. Kacmarcik, Z. Pribulova, C. Marcenat, T. Klein, P. Rodiere, L. Cario, and P. Samuely, Phys. Rev. B 82, 014518 (2010).

17

R. Friend and A. D. Yoffe, Adv. Phys. 36, 1 (1987).

18

H. Suhl, B. T. Matthias, and L. R. Walker, Phys. Rev.

Lett. 3, 552 (1959).

19

H. Choi, D. Roundy, H. Sun, M. Cohen, L. Louie, and G. Steven, Nature 418, 758 (2002).

20

I. I. Mazin and V. P. Antropov, Physica C 385, 49 (2003).

21

T. Yokoya, T. Kiss, A. Chainani, and S. et al., Science 294, 2518 (2001).

22

E. Boaknin, M. A. Tanatar, J. Paglione, D. Hawthorn, F. Ronning, R. W. Hill, M. Sutherland, L. Taillefer, J. Sonier, S. M. Hayden, et al., Phys. Rev. Lett. 90, 117003 (2003).

23

M. D. Johannes, I. I. Mazin, and C. A. Howells, Phys. Rev. B 73, 205102 (2006).

24

K. Onabe, M. Naito, and S. Tanaka, J. Phys. Soc. Jpn. 45, 50 (1978).

25

W. Fisher and M. Sienko, Inorg. Chem. 19, 39 (1980).

26

C. Van Degrift, Rev. Sci. Instrum. 46, 599 (1975).

27

P. Diener, P. Rodiere, T. Klein, C. Marcenat, J. Kacmar-cik, Z. Pribulova, D. J. Jang, H. S. Lee, H. G. Lee, and S. I. Lee, Phys. Rev. B 79, 220508 (2009).

28

R. Prozorov, R. W. Giannetta, A. Carrington, P. Fournier, R. L. Greene, P. Guptasarma, D. G. Hinks, and A. R. Banks, Appl. Phys. Lett. 77, 4202 (2000).

29

R. Prozorov, R. W. Giannetta, A. Carrington, F.M. Araujo-Moreira Phys. Rev. B 62, 115 (2000).

30

T. Klein, D. Braithwaite, A. Demuer, Phys. Rev. B 82, 184506 (2010).

31

B. Chandrasekhar and D. Einzel, Ann. Phys. 505, 535 (1993).

32

H. F. Hess, R. B. Robinson, and J. V. Waszczak, Phys. Rev. Lett. 64, 2711 (1990).

33

I. Guillamon, H. Suderow, S. Vieira, and P. Rodiere, Phys-ica C 468, 537 (2008).

34

F. Gygi and M. Schluter, Phys. Rev. Lett. 65, 1820 (1990).

35

the two set of Nb-bands called by Corcoran et al. 17 and 18, correspond respectively to 2 and 3 in Johannes and Mazin

36

P. Aynajian, T. Keller, L. Boeri, S. M. Shapiro, K. Habicht, and B. Keimer, Science 319, 1509 (2008).